prev

next

out of 47

View

219Category

## Documents

Embed Size (px)

Superconductivity

Peter SchmuserInstitut fur Experimentalphysik der Universitat Hamburg

AbstractLow-temperature superconductivity is treated at an introductory level. Thetopics include Meissner-Ochsenfeld effect and London equations, thermody-namic properties of the superconducting state, type I and II superconductors,flux quantisation, superconductors in microwave fields and superconductingquantum interference effects. Important experiments are discussed. The basicideas of the BCS theory and its implications are outlined.

1. INTRODUCTION

In these lectures I want to give an introduction into the physical principles of superconductivity and itsfascinating properties. More detailed accounts can be found in the excellent text books by W. Buckel[1] and by D.R. Tilley and J. Tilley [2]. Superconductivity was discovered [3] in 1911 by the Dutchphysicist H. Kamerlingh Onnes, only three years after he had succeeded in liquefying helium. During hisinvestigations on the conductivity of metals at low temperature he found that the resistance of a mercurysample dropped to an unmeasurably small value just at the boiling temperature of liquid helium. Theoriginal measurement is shown in Fig. 1. Kamerlingh Onnes called this totally unexpected phenomenonsuperconductivity and this name has been retained since. The temperature at which the transition tookplace was called the critical temperature Tc. Superconductivity is observed in a large variety of materialsbut, remarkably, not in some of the best normal conductors like copper, silver and gold, except at veryhigh pressures. This is illustrated in Fig. 2 where the resistivity of copper, tin and the high-temperaturesuperconductor YBa2Cu3O7 is sketched as a function of temperature. Table 1 lists some importantsuperconductors together with their critical temperatures at vanishing magnetic field.

Fig. 1: The discovery of superconductivity by Kamerlingh Onnes.

Fig. 2: The low-temperature resistivity of copper, tin and YBa2Cu3O7.

Table 1: The critical temperature of some common materials at vanishing magnetic field.

material Ti Al Hg Sn Pb Nb NbTi Nb3Sn

Tc [K] 0.4 1.14 4.15 3.72 7.9 9.2 9.2 18

A conventional resistance measurement is far too insensitive to establish infinite conductivity,a much better method consists in inducing a current in a ring and determining the decay rate of theproduced magnetic field. A schematic experimental setup is shown in Fig. 3. A bar magnet is insertedin the still normal-conducting ring and removed after cooldown below Tc. The induced current shoulddecay exponentially

I(t) = I(0) exp(t/)with the time constant given by the ratio of inductivity and resistance, = L/R, which for a normalmetal ring is in the order of 100 s. In superconducting rings, however, time constants of up to 105 yearshave been observed [4] so the resistance must be at least 15 orders of magnitude below that of copper andis indeed indistinguishable from zero. An important practical application of this method is the operationof solenoid coils for magnetic resonance imaging in the short-circuit mode which exhibit an extremelyslow decay of the field of typically 3 109 per hour [5].

Fig. 3: Induction of a persistent current in a superconducting ring.

There is an intimate relation between superconductivity and magnetic fields. W. Meissner and R.Ochsenfeld [6] discovered in 1933 that a superconducting element like lead completely expelled a weakmagnetic field from its interior when cooled below Tc while in strong fields superconductivity brokedown and the material went to the normal state. The spontaneous exclusion of magnetic fields uponcrossing Tc could not be explained in terms of the Maxwell equations and indeed turned out to be anon-classical phenomenon. Two years later, H. and F. London [7] proposed an equation which offereda phenomenological explanation of the Meissner-Ochsenfeld effect but the justification of the Londonequation remained obscure until the advent of the Bardeen, Cooper and Schrieffer theory [8] of super-conductivity in 1957. The BCS theory revolutionized our understanding of this fascinating phenomenon.It is based on the assumption that the supercurrent is not carried by single electrons but rather by pairs ofelectrons of opposite momenta and spins, the so-called Cooper pairs. All pairs occupy a single quantumstate, the BCS ground state, whose energy is separated from the single-electron states by an energy gapwhich in turn can be related to the critical temperature. The BCS theory has turned out to be of enormouspredictive power and many of its predictions and implications like the temperature dependence of the en-ergy gap and its relation to the critical temperature, the quantisation of magnetic flux and the existenceof quantum interference phenomena have been confirmed by experiment and, in many cases, even foundpractical application.

A discovery of enormous practical consequences was the finding that there exist two types ofsuperconductors with rather different response to magnetic fields. The elements lead, mercury, tin, alu-minium and others are called type I superconductors. They do not admit a magnetic field in the bulkmaterial and are in the superconducting state provided the applied field is below a critical field Hc whichis a function of temperature. All superconducting alloys like lead-indium, niobium-titanium, niobium-tinand also the element niobium belong to the large class of type II superconductors. They are charac-terized by two critical fields, Hc1 and Hc2. Below Hc1 these substances are in the Meissner phase withcomplete field expulsion while in the range Hc1 < H < Hc2 a type II superconductor enters the mixedphase in which magnetic field can penetrate the bulk material in the form of flux tubes. The Ginzburg-Landau theory [9] provides a theoretical basis for the distinction between the two types. Around 1960Gorkov [10] showed that the phenomenological Ginzburg-Landau theory is a limiting case of the BCStheory. Abrikosov [11] predicted that the flux tubes in a type II superconductor arrange themselves ina triangular pattern which was confirmed in a beautiful experiment by Essmann and Trauble [12]. In1962 Josephson [13] studied the quantum theoretical tunnel effect in a system of two superconductorsseparated by a thin insulating layer and he predicted peculiar and fascinating properties of such a Joseph-son junction which were all confirmed by experiment and opened the way to superconducting quantuminterference devices (SQUIDs) with extreme sensitivity to tiny magnetic fields.

2. MEISSNER-OCHSENFELD EFFECT AND LONDON EQUATION

We consider a cylinder with perfect conductivity and raise a magnetic field from zero to a finite value H .A surface current is induced whose magnetic field, according to Lenzs rule, is opposed to the appliedfield and cancels it in the interior. Since the resistance is zero the current will continue to flow withconstant strength as long as the external field is kept constant and consequently the bulk of the cylinderwill stay field-free. This is exactly what happens if we expose a lead cylinder in the superconductingstate (T < Tc) to an increasing field, see the path (a) (c) in Fig. 4. So below Tc lead acts as a perfectdiamagnetic material. There is, however, another path leading to the point (c). We start with a leadcylinder in the normal state (T > Tc) and expose it to a field which is increased from zero to H . Eddycurrents are induced in this case as well but they decay rapidly and after a few hundred microsecondsthe field lines will fully penetrate the material (state (b) in Fig. 4). Now the cylinder is cooled down.At the very instant the temperature drops below Tc , a surface current is spontaneously created and themagnetic field is expelled from the interior of the cylinder. This surprising observation is called the

Meissner-Ochsenfeld effect after its discoverers; it cannot be explained by the law of induction becausethe magnetic field is kept constant.

Fig. 4: A lead cylinder in a magnetic field. Two possible ways to reach the superconducting final state with H > 0 are sketched.

Ideally the length of the cylinder should be much larger than its diameter to get a vanishing demagnetisation factor.

In a (T,H) plane, the superconducting phase is separated from the normal phase by the curveHc(T ) as sketched in Fig. 5. Also indicated are the two ways on which one can reach the point (c). Itis instructive to compare this with the response of a normal metal of perfect conductivity. The fieldincrease along the path (a) (c) would yield the same result as for the superconductor, however thecooldown along the path (b) (c) would have no effect at all. So superconductivity means definitelymore than just vanishing resistance.

Fig. 5: The phase diagram in a (T, H) plane.

I have already used the terms superconducting phase and normal phase to characterize thetwo states of lead. These are indeed phases in the thermodynamical sense, comparable to the differentphases of H2O which is in the solid, liquid or gaseous state depending on the values of the parameterstemperature and pressure. Here the relevant parameters are temperature and magnetic field (for somematerials also pressure). If the point (T,H) lies below the curve Hc(T ) the material is superconductingand expels the magnetic field, irrespective of by which path the point was reached. If (T,H) is abovethe curve the material is normal-conducting.

The first successful explanation of the Meissner-Ochsenfeld effect was achieved in 1935 by Heinzand Fritz London. They assumed that the supercurrent is carried by a fraction of the conduction electronsin the metal. The super-electrons experience no friction, so their equation of motion in an electric fieldis

me~v

t= e ~E .